Presentation on theme: "Nanostructured self-assembled P3HT thin films and their application to enhance organic solar cell efficiency Varun Vohra 1,Hideyuki Murata 2 1 University."— Presentation transcript:
Nanostructured self-assembled P3HT thin films and their application to enhance organic solar cell efficiency Varun Vohra 1,Hideyuki Murata 2 1 University of Electro-Communications (UEC), Japan 2 Japan Advanced Institute of Science and Technology (JAIST), Japan 4th International Conference on Nanotek and Expo (Nanotek-2014) San Francisco, USA December 1 st, 2014
Introduction: Nanostructured films of P3HT S. Zhu et al. in Nature 400, 49-51(1999) Phase separated polymer blends studied since over a decade Mostly electronically inactive blends (e.g. PS-PMMA) Methods to obtain nanostructured thin films of P3HT: Nanolithography M. Aryal et al. in ACS Nano 3, 3085-3090 (2009) Elaborated chemistry K. Sivanandan et al. in Macromolec. 43, 233-241 (2010) Can we obtain similar structures using commercially available polymer blends?
Simple idea to form nanostructured P3HT Phase separation between P3HT and commercially available polymer materials Example of nanoporous structures obtained from P3HT:PS blends before and after selective removal of PS (structure already formed prior to PS removal)
P3HT nanoporous and nanoisland films Two types of structure can be fabricated with PS Focus on nanoporous films
Tuning the pore dimensions / morphology Method 1: Changing the molecular weight of the polymers Increasing polystyrene molecular weight Method 2: Changing the P3HT:PS ratio Increasing polystyrene wt % (15 to 50 wt%) Combination of the two methods: Pore diameters can be tuned from 100 to 650 nm
Large scale nanostructured film formation? 5 m x 5 m Uniform samples (small exception at the edges) Sample size: 2.5 cm x 2.5 cm 20 m x 20 m 100 m x 100 m What can we use these porous films for?
Potential applications Organic solvent extraction vacuum Solvent + water + impurities Solvent + water + impurities Solvent Si wafer Au SiO 2 Increased sensitivity of P3HT based OFET sensors Sensing surface Si wafer Au SiO 2 Increased sensing surface Increased donor-acceptor interface in organic solar cells
Interdigitated Diffusive Bilayer by Sequential deposition Ideal morphology for polymer solar cells Efficient charge transport to their respective electrodes Less charge generation in planar bilayers Efficient charge generation Unefficient charge collection Can we increase the charge generation through nanostructured donor-acceptor interfaces?
Morphology of the nanoporous films In addition to increased Jsc, we should observe increased FF AFM measurements: underlying non structured P3HT buffer layer Angle dependent FTIR: organization of the P3HT chains at the P3HT-PS interface PEDOT:PSS
1/ Deposition of PCBM from dichloromethane 2/Removal of PCBM with cyclohexanone 1/ filling the pores with PCBM and allowing diffusion of PCBM into P3HT pore depth decreases from 60 to 15 nm (PS 25wt% after PS removal) 2/ removing the PCBM and the parts of P3HT containing a high concentration of (diffused) PCBM widening : +75 nm on each sides deepening: +60 nm Lateral diffusion > Vertical diffusion: Confirms the different orientations! Different orientations in the bulk and the surface
PS (wt%) Jsc* (mA/cm 2 ) Voc (V) FF (%) (%) Rs (Ω/cm 2 ) Wetting layer Absorption ratio (A/A 0 ) 010.8 0.57412.517.04130 nm1 1510.2 12.30.60462.778.27104 nm0.832 2510.5 14.10.61513.254.6176 nm0.745 3510.0 15.60.61493.024.1863 nm0.640 Increase in corrected Jsc, Voc, FF and consequently PCE *Jsc corresponds to the measured Jsc divided by the absorption ratio Photovoltaic parameters
Origins of the increase in device performances PEDOT:PSS 1 2 1 2 Planar bilayer nanostructured bilayer: increase in donor-acceptor interface P3HT crystallite reorientation : better hole transport properties reduced Rs increased Voc and FF Thin P3HT buffer layer (no PCBM):nanostructured p-i-n junction further increases FF PS (wt%) Jsc* (mA/cm 2 ) Voc (V) FF (%) (%) Rs (Ω/cm 2 ) Wetting layer Absorption ratio (A/A 0 ) 010.8 0.57412.517.04130 nm1 2510.5 14.10.61513.254.6176 nm0.745
Easy and cost effective method to prepare spin-coated nanostructured P3HT films from blends of commercially available polymers (P3HT + PS) Tuning of pore dimensions can be controlled by wt% and Mw Nanoscale phase separation induces reorientation of the polymer crystallites at the P3HT/PS interface Nanostructured diffusive bilayer solar cells have an average PCE of upto 3.25% (30% increase with respect to the planar equivalent) A deeper analysis of the active layer morphology is necessary to understand the increase in PV performances Summary The nanostructured thin films have potential for various applications Feel free to come and exchange ideas The nanostructured thin films have potential for various applications Feel free to come and exchange ideas
Organic solar cells based on nanoporous P3HT obtained from self-assembled P3HT:PS templates V. Vohra, M. Campoy-Quiles, M. Garriga, H. Murata, J. Mater. Chem., 2012,22, 20017-20025 Nanostructured P3HT films with tunable dimensions through self-assembly with PS V. Vohra, O. Notoya, T. Huang, M. Yamaguchi, H. Murata, Polymer, 2014, 55, 2213-2219 An international collaboration Hideyuki Murata Masayuki Yamaguchi Osamu Notoya Tong Huang Varun Vohra Mariano Campoy-Quiles Miguel Garriga Xiaojun Guo (future projects) On-going and future collaborations: Very open to new collaboration and projects
Energy related research!! Energy related re...zzearch Ener...zzzzzy
Your consent to our cookies if you continue to use this website.